Le logiciel Cerius2 et le champ de force UFF ont été utilisés afin de mener l’étude de l’intercalation du monomère e-caprolactone et du polymère poly(e-caprolactone) au sein de feuillet d’argile de type Montmorillonite. Ces travaux ont fait l’objet de deux publications et d’une communication orale.
3. a) P. Ewald, Ann. Phys. 1921, 64, 253-287. b) N. Karasawa, W.A. Goddard III, J. Phys. Chem. 1989, 93, 7320-7327.
Molecular Dynamics Study of E-Caprolactone Intercalated
in Wyoming Sodium Montmorillonite
Anouk Gaudel-Siri,†,‡Patrick Brocorens,†Didier Siri,§ Fabrice Gardebien,†
Jean-Luc Bre´das,†,|and Roberto Lazzaroni*,†
Service de Chimie des Mate´riaux Nouveaux, Universite´de Mons-Hainaut, 20 Place du Parc, B-7000 Mons, Belgium, Laboratoire Re´So-UMR 6516, Universite´d’Aix-Marseille 3, Faculte´
St.Je´roˆme, Av. Esc. Normandie-Niemen, 13397 Marseille Cedex 20, France, Laboratoire de Chimie The´orique et Mode´lisation Mole´culaire, CNRS-UMR 6517, Universite´sd’Aix-Marseille
1et 3, Faculte´St.Je´roˆme, Av. Esc. Normandie-Niemen, 13397 Marseille Cedex 20, France, and School of Chemistry and Biochemistry, Georgia Institute of Technology,
Atlanta, Georgia 30332-0400
Received March 21, 2003. In Final Form: July 14, 2003
The intercalation process of the ϵ-caprolactone monomer into sodium montmorillonite clay is modeled with a combined molecular mechanics/molecular dynamics approach. This study is aimed at understanding the initial stages of caprolactone polymerization within the channels of the clay, to form highly dispersed nanocomposites. The theoretical method is first validated by modeling dry and hydrated Wyoming sodium montmorillonite; the caprolactone-intercalated clay is then investigated, with particular emphasis on the energetics of the intercalation process and the nature of the interactions building up between the organic molecules and the channel walls and sodium counterions.
Poly(ϵ-caprolactone) (PCL) is a biodegradable aliphatic polyester that is being intensively investigated for use in medical devices and degradable packaging. However, the mechanical properties of the PCL homopolymer are too poor to allow its direct use. To improve the mechanical properties and thermal stability, nanocomposites based on PCL and layered aluminosilicates (montmorillonite-type clay) represent a valuable alternative. Because of the dispersion of nanometer-size clay sheets, nanocom-posites exhibit new and improved properties compared to microcomposites or filled polymers.1,2
Polymer nanocomposites are usually prepared by melt intercalation; in that procedure, alkali-metal cations of the clay must first be replaced by organic surfactants in order to render the clay channels more organophilic and to allow the intercalation of the polymer. The physico-chemical parameters governing the intercalation process and the influence of the organic counterions on the stability of the nanocomposites have been extensively investigated by model calculations (see refs 3-5 and references therein). Those studies allow for the a priori design of composite materials with a well-defined microstructure.
Remarkably, the need for those organophilic counterions can be circumvented if the polymer is directly generated
within the channels. It has been shown recently that the ϵ-caprolactone monomers (CL) spontaneously intercalate at ambient temperature between Na-montmorillonite sheets.6Subsequent polymerization involving the inter-calated monomers then leads to composites with excellent dispersion of the clay sheets in the matrix. To exploit best this new route to polymer nanocomposites, it is essential to obtain a molecular scale description of the intercalation process for the monomer. Through a molecular modeling approach, this study aims at shedding light on (i) the structure of the intercalated system, that is, the spatial distribution of the CL molecules with respect to the clay walls and the counterions, and (ii) the nature of inter-molecular interactions favoring intercalation. In turn, this will allow an understanding of whether the spontaneous intercalation of the monomer (and the subsequent po-lymerization leading to the nanocomposite) is specific to caprolactone, or this new route could be extended to the preparation of other polymer/Na-montmorillonite nano-composites.
Here we focus on the modeling of the CL-intercalated Na-montmorillonite system. Montmorillonite belongs to the family of 2:1 phyllosilicates. Their crystal structure consists of layers of two silica tetrahedral sheets fused to an edge-shared octahedral sheet of aluminum hydroxide. Stacking of the layers leads to a regular van der Waals gap or interlayer. Isomorphic substitutions within the layers (silicon replaced by aluminum in the tetrahedral sheets and aluminum replaced by magnesium in the octahedral sheet) generate negative charges that are counterbalanced by cations residing in the interlayer region. The natural form of Wyoming montmorillonite contains hydrated Na+or K+cations. The layer charge of montmorillonite clays is usually between-0.5eand-1.2
eper O20(OH)4formula unit cell, and octahedral substitu-tions are responsible for about2/3of the total charge. We * To whom correspondence should be addressed. E-mail:
†Service de Chimie des Mate´riaux Nouveaux, Universite´ de Mons-Hainaut.
‡Laboratoire Re´So- UMR 6516, Universite´ d’Aix-Marseille 3. §Laboratoire de Chimie The´orique et Mode´lisation Mole´culaire, CNRS-UMR 6517, Universite´s d’Aix-Marseille 1 et 3.
|School of Chemistry and Biochemistry, Georgia Institute of Technology.
(1) (a) Krishnamoorti, R.; Vaia, R. A.; Giannelis, E. P.Chem. Mater. 1996,8, 1728. (b) Giannelis, E. P.Adv. Mater.1996,8, 29.
(2) Alexandre, M.; Dubois, P.Mater. Sci.Eng. 2000,R28, 1. (3) Vaia, R. A.; Giannelis, E. P.Macromolecules1997,30, 8000. (4) Giannelis, E. P.; Krishnamoorti, R.; Manias, E.Adv. Polym. Sci. 1999,138, 107.
(5) Balazs, A. C.; Singh, C.; Zhulina, E.; Lyatskaya, Y.Acc. Chem. Res. 1999,8, 651.
(6) (a) Lepoittevin, B.; Devalckenaere, M.; Pantoustier, N.; Alexandre, M.; Kubies, D.; Calberg, C.; Jeroˆme, R.; Dubois, P.Polymer2002,43, 4017. (b) Lepoittevin, B.; Devalckenaere, M.; Alexandre, M.; Pantoustier, N.; Calberg, C.; Jeroˆme, R.; Dubois, Ph.Macromolecules2002,35, 8385. 8287 Langmuir 2003, 19, 8287-8291
10.1021/la034491n CCC: $25.00 © 2003 American Chemical Society Published on Web 08/27/2003
here consider the unit cell formula Na0.75(Si7.75Al0.25 )-(Al3.5Mg0.5)O20(OH)4which represents a mineral with a charge of-0.75e. This particular clay is chosen because of its wide use in the preparation of polymer nanocom-posites.
Molecular dynamics (MD) simulations are performed to obtain information on the geometrical aspects of the intercalation process and to collect average data about the interlayer species. As a preliminary step aimed at evaluating the reliability of our approach, dry montmo-rillonite is simulated and our results for this system are compared to previous theoretical and experimental stud-ies.7 We then proceed to the simulation of the CL-intercalated system; the results are analyzed in terms of the orientation of the CL molecules in the interlayer channel, their interaction with the Na+cations, and the energetics of the intercalated system.
2. Computational Methodology
For this study, we used the molecular dynamics module and the energy minimizer of the Cerius24.0 package.8 Due to the presence of organic and inorganic species, the universal force field (UFF)9was selected.
2.1. Caprolactone Molecule. The geometry of the isolated CL molecule was optimized with the UFF. During the energy minimization, the partial charges of the atoms were optimized with the QEq algorithm;10 they are reported in Table 1. As found in previous experimental and theoretical studies,11the seven-membered ring of CL preferentially adopts a chair conformation (Figure 1).
2.2. Dry Na-Montmorillonite. The simulation system consists of a periodically replicated, rectangular box that contains eight Na-montmorillonite unit cells (4 × 2 × 1). The dimensions of the starting box area) 20.8 Å, b ) 18.4 Å, andc) 12.0 Å. The starting system is monoclinic
with β ) 99°, as in the unit cell of dry montmorillonite.12 The positions and charges of the sites in the unit cell of the clay are directly derived from the empirical model introduced by Skipper et al.7a(Table 1): four isomorphous substitutions of trivalent Al atoms by divalent Mg atoms in the octahedral sheet and two isomorphous substitutions of tetravalent Si atoms by trivalent Al atoms in the tetrahedral sheets. Six Na+counterions are placed in the interlayer region.
2.3. Na-Montmorillonite with Intercalated CL Molecules. In a preliminary MD study of hydrated Na-montmorillonite with the UFF, we have found that the density of water in the interlayer region (0.95) is very close to the density of liquid water. On that basis, we assume that the density of CL between the clay sheets is close to the density of liquid CL (1.03). Moreover, X-ray diffraction data6a provide the d001 parameter of Na-montmorillonite with intercalated CL molecules (19.6 Å). If we subtract the volume of the simulation cell of dry Na-montmorillonite at equilibrium (3735 Å3) from the calculated volume of a monoclinic Na-montmorillonite withd001) 19.6 Å (7410 Å3), we obtain a volume of 3675 Å3occupied by CL molecules. With a density of 1.03, this corresponds to about 18 CL molecules in the simulation cell. Therefore, for the simulation of the CL-intercalated system, the starting point is the monoclinic system of dry Na-montmorillonite, with thecparameter enlarged to 20.0 Å and 18 CL monomer molecules inserted in the interlayer spacing. Let us recall that since the polymerization of caprolactone is most efficient when the medium is anhydrous, the clay is usually dried before the monomer incorporation.6 Therefore, water-free montmorillonite appears to be the most suitable system to model CL intercalation.
2.4. Molecular Dynamics Simulations. For the two periodic systems (dry and CL-intercalated Na-montmo-rillonite), the configuration of the starting simulation cell is replicated in all three spatial directions through periodic boundary conditions. Ewald summation methods13are used to treat Coulombic and attractive van der Waals interactions with a standard cutoff. Repulsive van der Waals interactions are directly calculated with standard parameters. All simulations are performed at a constant temperature using a “weak coupling” algorithm14and a coupling time constant of 500 fs. The Verlet algorithm and a time step of 1 fs are used for all dynamics simulations.
To reduce the computational effort, we impose that the atoms in the clay sheets remain at constant positions during the MD calculation, as the sheets are expected to (7) (a) Skipper, N. T.; Refson, K.; McConnell, J. D. C.J. Chem. Phys.
1991,94, 7434. (b) Karaborni, S.; Smit, B.; Heidug, W.; Urai, J.; Oort, E. v.Science1996,271, 1102. (c) Young, D. A.; Smith, D. E.J. Phys. Chem. B2000,104, 9163. (d) Park, S.-H.; Sposito, G.J. Phys. Chem. B2000,104, 4642. (e) Chavez-Paez, M.; Van Workum, K.; de Pablo, L.; de Pablo, J. J.J. Chem. Phys.2001,114, 1405.
(8) Molecular Simulations Inc., 9685 Scranton Road, San Diego, CA; 1997.
(9) (a) Rappe´, A. K.; Casewit, C. J.; Colwell, K. S.; Goddard, W. A., III; Skiff, W. M.J. Am. Chem. Soc.1992,114, 10024. (b) Casewit, C. J.; Colwell, K. S.; Rappe´, A. K.J. Am. Chem. Soc.1992,114, 10035. (b) Casewit, C. J.; Colwell, K. S.; Rappe´, A. K.J. Am. Chem. Soc.1992,114, 10046.
(10) Rappe´, A. K.; Goddard, W. A., IIIJ. Phys. Chem.1991,95, 3358. (11) (a) Abraham, R. J.; Ghersi, A.; Petrillo, G.; Sancassan, F.J. Chem. Soc., Perkin Trans. 21997, 1279. (b) Allen, F. H.; Howard, J. A. K.; Pitchford, N. A.; Vinter, J. G.Acta Crystallogr., Sect. B1994, 382.
(12) Brindley, G. W.; Brown, G.Crystal Structures of Clay Minerals and Their X-ray Identification; Mineralogical Society: London, 1980. (13) Karasawa, N.; Goddard, W. A., IIIJ. Phys. Chem.1989,93, 7320.
(14) Berendsen, H. J. C.; Postma, J. P. M.; van Gunsteren, W. F.; DiNola, A.; Haak, J. R.J. Chem. Phys.1984,81, 3684.
Table 1. Atomic Chargesa atom C1 C2 C3 C4 C5 O6 C7 O8 H9 charge/e -0.20 -0.28 -0.28 -0.24 0.00 -0.52 0.64 -0.47 0.13 atom H10 H11 H12 H13 H14 H15 H16 H17 H18 charge/e 0.10 0.16 0.13 0.14 0.14 0.18 0.10 0.14 0.12 atom Si Alb Mg O (OH) H O (bridge) O charge/e 1.2 3.0 or 0.2 2.0 -1.424 0.424 -1.0 -0.8
aFor the CL molecule, atomic charges are optimized with the QEq algorithm; for montmorillonite, they are assigned according to the method due to Skipper et al. (ref 7a).bThe partial charge of the Al atoms is 3.0 in the octahedral sites and 0.2 when they replace a Si atom in the tetrahedral sheet.
Figure 1. Atom numbering and chair conformation of the CL molecule.
be fully rigid. However, as a consequence,NPT dynamics simulations (i.e., performed at constant number of par-ticles, pressure, and temperature) are not possible (since the volume would be allowed to change) and we have to carry out successive, alternatingNVT dynamics simula-tions and energy minimization steps, also using the UFF. DuringNVT dynamics simulations, the clay sheets are immovable, but when energy minimizations are per-formed, registry and swelling motions are allowed. The “smart minimizer” of the Cerius2package is used with 2500-5000 iterations. The RMS-force criterion is 0.005 kcal mol-1Å-1, the criterion on the energy difference is 10-5kcal mol-1, and the criterion on the RMS-shift is 3 × 10-5Å.
For the clay with intercalated CL molecules, a procedure in three steps is followed:
(1) The initial optimization of the cell parametercleads to a value of 19.4 Å. Then, the cell parameters are frozen and shortNVT dynamics simulations (20 ps) are performed at increasing temperatures from 300 to 600 K in incre-ments of 50 K. This first step allows the system to overcome potential barriers and rearrange itself into a state with improved interactions among CL molecules, between Na+ cations and CL molecules, and between the clay sheets and CL molecules at a starting cell parametercof 19.4 Å.
(2)NVT dynamics simulations (20 ps) at 300 K alternate with energy minimizations in order to optimize the interlayer spacing. At first, the cell parameter cis the only degree of freedom. As soon ascis optimized in the monoclinic space group (c) 18.3 Å), registry motions are allowed: two degrees of freedom (R and β) are added. Therefore, the three parametersR, β, and care simul-taneously optimized and the equilibrium configuration is obtained. This step-by-step strategy prevents the system from evolving toward irrelevant and less stable configu-rations with a large sliding of the two clay sheets.
(3) We start from the equilibrium configuration found in step 2, and aNVT dynamics simulation of 460 ps is performed at 300 K. We observe that the system reaches equilibration after 50 ps; then average data are collected over 410 ps.
For dry Na-montmorillonite, steps 1 and 2 lead to the equilibrium configuration.
3. Results and Discussion
3.1. Dry Na-Montmorillonite. From this dynamics study with the UFF, we obtaind001) 9.88 Å, R ) 97°, and β ) 95° for the equilibrium configuration (Figure 2). These results are very close to experimental data (9.55< d001< 9.8( 0.1 Å, R ) 90°, and β ) 99°) and previous MD and Monte Carlo calculations (9.7< d001< 9.8 Å).7This clearly demonstrates the validity of our theoretical approach. We only note a slight registry motion of the clay sheets since R and β differ from the starting values. In agreement with previous studies, the equilibrium position of Na+cations is in the hexagonal sites, where the cation is nestled within two hexagonal cavities of opposite tetrahedral sheets (Figure 2b). Most of the Na+cations are 6 Å apart, but two of them, which are close to the isomorphic substitution of a Si atom, are only 5.0 Å apart (Figure 2b). From the analysis of the different energy terms, it appears that the stability of the clay is mainly due to electrostatic interac-tions.
3.2. Na-Montmorillonite with Intercalated CL Molecules. As a preliminary step to investigate the orientational behavior of the molecules, we placed 6 CL molecules in the interlayer spacing with different starting
orientations relative to the clay sheets. Short MD simula-tions led to a similar orientation, with the CL rings preferentially oriented to maximize their interaction with the clay sheets, that is, the chair is roughly parallel to the surface of the sheet. Therefore, when considering the “fully loaded” system, the 18 CL molecules form two layers, roughly parallel to the channel walls. The Na+counterions are distributed between the CL layers and the clay sheets. During MD simulations, the geometry of the CL rings is allowed to change but the partial charges are fixed.
From these calculations, we obtaind001) 18.17 Å, R ) 87.6°, and β ) 100.8° for the equilibrium configuration (Figure 3). We find a slight registry motion of the clay sheets for this system as well. The volume of the box is 6824 Å3, implying that the remaining volume for CL molecules is 3090 Å3. This corresponds to a density of 1.10 for the interlayer phase (close to the density of liquid CL). Figure 2. Equilibrium configuration of dry Na-montmorillo-nite. Only the Na+cations are shown with their van der Waals radius. (a) Side view with the atoms of the clay sheets in a “ball and stick” representation. (b) Top view. Only the SiO3moieties (sticks) of the tetrahedral sheets surrounding the Na+cations are shown.
Figure 3. Equilibrium configuration of Na-montmorillonite intercalated with CL molecules.
The average intercalation energy of a CL molecule in the interlayer spacing of dry Na-montmorillonite is defined as
U(18) and U(0) are the equilibrium configuration potential energies of intercalated and dry Na-montmorillonite, respectively; andU(CL) is the potential energy of one CL molecule. We find a large negative value for ∆U (-35.9 kcal mol-1). We have to subtract from that value the solvation energy of CL, which is included inU(18) but not in U(CL); from a calculation on a cluster of 18 CL molecules, it is estimated to be around 20 kcal mol-1. Therefore, the global stabilization upon intercalation is around 16 kcal mol-1per molecule, which indicates that from the energetic point of view, the spontaneous inter-calation of CL molecules in Na-montmorillonite is highly favorable. The entropy balance of the intercalation process cannot be estimated from our calculations. However, for a similar system (polystyrene intercalated in montmo-rillonite channels), Vaia and Giannelis3,4have performed detailed mean-field studies to evaluate the energetic and entropic aspects of the intercalation process. They have shown that the loss of conformational freedom of the molecules upon intercalation can be compensated by the entropic gain of the ions present in the cavity, due to the increase in the clay sheet separation. In particular, this compensation is complete (i.e., the entropic balance is neutral) when the gallery height increases by less than 1 nm, as is the case in our systems. Those results have been obtained for alkylammonium counterions; the same compensating effect must be at work in the Na-containing compounds studied here, even though to a significantly smaller extent (because the Na+cations tend to remain close to the channel walls, see below). Nevertheless, the entropic balance is expected not to be strongly unfavorable in our systems. This, combined with a clear energetic stabilization, is consistent with the observation of spon-taneous intercalation.
To gain information on (i) the spatial distribution of the various species within the channels and (ii) the nature of the interactions among those species, average positional data are collected during the late stages of the MD simulations, after the system has reached equilibration. Radial distribution functions are calculated between Na+ cations and the oxygen atoms of CL molecules in order to estimate the solvation of Na+cations by CL molecules; the interaction between Na+cations and the oxygen atoms of the clay is evaluated as well. Radial distribution functions are defined as follows:
where dnris the number of B particles in a shell between r and r+ dr around each A particle and FBis the density of B particles. The number of nearest neighbors is deduced from the radial distribution function:
where the cutoff is defined in order to consider only the first peak of the radial distribution function. The results are reported in Figure 4.
On average, the first solvation shell of Na+cations is composed of 3 carbonyl oxygen atoms (d(Na-O) ) 2.29 Å) and 1.6 intracyclic oxygen (d(Na-O) ) 2.25 Å) from CL
molecules and 2 oxygen atoms from the silicate sheets (d(Na-O) ) 2.27 Å). In terms of coordination number, these results are quite similar to those of recent calcula-tions15dealing with the hydration of Na+cations (5 or 6 water molecules in the first solvation shell). The ability of CL molecules to solvate the Na+cations in the interlayer spacing is therefore likely an important factor contributing to the spontaneous intercalation process.
Density profiles of the interlayer species are determined through calculations of their probability distribution (15) (a) Degre`ve, L.; Quintale, C., Jr.J. Chem. Phys.1994,101, 2319. (b) Obst, S.; Bradaczek, H.J. Phys. Chem.1996,100, 15677. (c) Lee, S. H.; Rasaiah, J. C.J. Phys. Chem.1996,100, 1420. (d) Koneshan, S.; Rasaiah, J. C.; Lynden-Bell, R. M.; Lee, S. H.J. Phys. Chem. B1998, 102, 4193. (e) White, J. A.; Schwegler, E.; Galli, G.; Gygi, F.J. Chem. Phys.2000,113, 4668.
∆U ) [U(18) - U(0) - 18U(CL)]/18
gAB(r)) dnr 4πFBr2dr
Figure 4. Radial distribution functions around Na+cations for (A) the carbonyl oxygen atoms of CL, (B) the intracyclic oxygen atoms of CL, and (C) the clay oxygen atoms.
functions in the z direction, that is, the direction per-pendicular to the plane of the clay sheet (Figure 5). Na+ cations are distributed close to the clay sheets, while the
CL molecules form two layers with various orientations of the carbonyl and intracyclic oxygen atoms. The dis-tribution of the Na+cations is not symmetric: four cations are close to the first clay sheet while only two are close